fabrication with combined computer-aided design and 3D .... The incongruence between the computer-aided ... The same dental technician at the commercial ...
RESEARCH AND EDUCATION
Die spacer thickness reproduction for central incisor crown fabrication with combined computer-aided design and 3D printing technology: An in vitro study Lisa N. Hoang, DMD, MS,a Geoffrey A. Thompson, DDS, MS,b Seok-Hwan Cho, DDS, MS, MS,c David W. Berzins, BS, PhD,d and Kwang Woo Ahn, PhDe Clearance is needed between a ﬁxed restoration and the prepared tooth to provide space for the luting agent. Methods such as venting, axial grooves, and provision of axial cement space have been used to reduce the hydraulic pressure between the cement and cast restoration and therefore improve seating, decrease seating time, and allow the escape of excess cement.1-8 The application of paint-on die spacer before waxing is one of the most popular methods for providing this space.3,9 Die spacers have been used in ﬁxed dental prostheses for many years.3,10-13 Die spacer has been shown to improve the marginal ﬁt between the restoration and tooth preparation, decreasing the risk of cement dissolution, plaque accumulation, recurrent caries, and periodontal problems.14 The thickness of
ABSTRACT Statement of problem. The inability to control die spacer thickness has been reported. However, little information is available on the congruency between the computer-aided design parameters for die spacer thickness and the actual printout. Purpose. The purpose of this study was to evaluate the accuracy and precision of the die spacer thickness achieved by combining computer-aided design and 3-dimensional printing technology. Material and methods. An ivorine maxillary central incisor was prepared for a ceramic crown. The prepared tooth was duplicated by using polyvinyl siloxane duplicating silicone, and 80 die-stone models were produced from Type IV dental stone. The dies were randomly divided into 5 groups with assigned die spacer thicknesses of 25 mm, 45 mm, 65 mm, 85 mm, and 105 mm (n=16). The printed resin copings, obtained from a printer (ProJet DP 3000; 3D Systems), were cemented onto their respective die-stone models with self-adhesive resin cement and stored at room temperature until sectioning into halves in a buccolingual direction. The internal gap was measured at 5 deﬁned locations per side of the sectioned die. Images of the printed resin coping/die-stone model internal gap dimensions were obtained with an inverted bright ﬁeld metallurgical microscope at ×100 magniﬁcation. The acquired digital image was calibrated, and measurements were made using image analysis software. Mixed models (a=.05) were used to evaluate accuracy. A false discovery rate at 5% was used to adjust for multiple testing. Coefﬁcient of variation was used to determine the precision for each group and was evaluated statistically with the Wald test (a=.05). Results. The accuracy, expressed in terms of the mean differences between the prescribed die spacer thickness and the measured internal gap (standard deviation), was 50 mm (11) for the 25 mm group simulated die spacer thickness, 30 mm (10) for the 45 mm group, 15 mm (14) for the 65 mm group, 3 mm (23) for the 85 mm group, and -10 mm (32) for the 105 mm group. The precision mean of the measurements, expressed as a coefﬁcient of variation, ranged between 14% and 33% for the 5 groups. Conclusions. For the accuracy evaluation, statistically signiﬁcant differences were found for all the groups, except the group of 85 mm. For the precision assessment, the coefﬁcient of variation was above 10% for all groups, showing the printer’s inability to reproduce the uniform internal gap within the same group. (J Prosthet Dent 2015;113:398-404)
Supported by an American Academy of Fixed Prosthodontics Stanley D. Tylman research grant (02600-74716) and the Marquette University School of Dentistry Student Research Fund. a Resident, Graduate Prosthodontics, Marquette University School of Dentistry, Milwaukee, Wis. b Assistant Professor and Director, Department of General Dental Sciences, Graduate Prosthodontics, Marquette University School of Dentistry, Milwaukee, Wis. c Assistant Professor and Director, Predoctoral Prosthodontics and Biomaterials, Department of General Dental Sciences, Marquette University School of Dentistry, Milwaukee, Wis. d Associate Professor and Director, Department of General Dental Sciences, Graduate Dental Biomaterials, Marquette University School of Dentistry, Milwaukee, Wis. e Assistant Professor, Division of Biostatistics, Medical College of Wisconsin, Milwaukee, Wis.
THE JOURNAL OF PROSTHETIC DENTISTRY
Clinical Implications The incongruence between the computer-aided design program setting and the actual coping printout negatively affect the clinical ﬁt of the deﬁnitive restoration.
this die spacer affects the fracture strength of a ceramic restoration, its retention, and the marginal gap.1,2,15,16 According to Tuntiprawon and Wilson,15 ceramic crowns displayed a greater fracture strength when the mean internal gap at the axial wall was less than 73 mm. A lower failure strength was reported when the mean internal gap was greater than 122 mm without any signiﬁcant improvement in seating. Conﬂicting results have been reported on the inﬂuence of die spacer thickness on retention. Eames et al1 reported a 25% increase in retention when comparing 0 mm to 25 mm die spacer thickness. This improved retention was supported by Carter and Wilson,2 who reported that retention increased from 250 N to 375 N as die spacer thickness changed from 0 to 8 layers. In contrast, Jorgensen and Esbensen16 reported a moderate association between ﬁlm thickness and retention, while Vermilyea et al17 reported a 32% reduction in retention when comparing 0 with 2 layers of Tru-Fit paint on die spacer (George Taub Products and Fusion Co Inc). There is greater consistency when evaluating the cause and effect relationship of die spacer thickness and marginal gap.2-4 The magnitude of the marginal gap observed without the use of die spacer was as high as 649 mm3. The marginal gap was signiﬁcantly improved from 479 mm to 38 mm as the die spacer thickness was increased from 1 to 8 layers.1-3 Marginal gap can also be inﬂuenced by the marginal design and total occlusal convergence of the preparation.18,19 McLean and von Fraunhofer18 showed that the best marginal gap was obtained with chamfer or rounded shoulder marginal design when compared with straight shoulder marginal design. The maximum tolerated marginal gap was 120 mm for ceramic crowns. Hollenback20 suggested an ideal die spacer thickness of 25 mm, which corresponds to the ﬁlm thickness of Type I zinc phosphate cements. However, studies with commercially available paint-on die spacer products have shown inconsistent results.5,13,21,22 Computer-aided design (CAD) technology provides the ability to virtually design restorations and program the die spacer thickness. The virtual coping can be produced by milling23,24 or rapid prototyping. Rapid prototyping uses the layer-to-layer fabrication of 3-dimensional physical models directly from CAD data.25-27 Rapid prototyping is further subdivided into stereolithography, selective layer sintering, fused deposition modeling, laminated object
Hoang et al
manufacturing, and 3D printing technology (3DPT).28 3DPT is used for copings, partial ﬁxed dental prostheses, anatomic contour pressable patterns, and partial removable dental prosthesis frameworks, which are formed in either wax or acrylic resin.29 Accuracy is deﬁned to assess the degree of closeness of the internal gap measurements to the reference values (programmed die spacer thicknesses). Therefore, the purpose of this study was to evaluate the accuracy and precision of the die spacer thickness achieved by combining CAD and 3DPT to test the accuracy of CAD/ 3DPT by comparing various measured internal gap thicknesses with the prescribed values of 25 mm, 45 mm, 65 mm, 85 mm, and 105 mm. The accuracy null hypothesis was that no overall difference would be found between the CAD/3DPT achieved internal gap thicknesses and the prescribed die spacer thicknesses. The secondary objective of the research was to measure the printer’s ability to reproduce the uniform die spacer thickness for all the specimens within an assigned die spacer thickness group. A statistical analysis was performed to test whether there was difference among the varying die spacer thicknesses and the reproducibility of the printer. The coefﬁcient of variation (CV) was adopted to determine the precision of the measurements. Ten percent of CV has been widely used as cutoff to deﬁne high precision.30-32 Therefore, the null hypothesis for precision was that the CV was equal to 10% because a CV less than 10% was considered reasonable.30-32 MATERIAL AND METHODS An ivorine maxillary central incisor (T1560; Columbia Dentoform Corp) was prepared to receive a ceramic crown restoration with the following features: a total convergence angle of 12 degrees, an incisal reduction of 2 mm, a uniform axial reduction of 1.5 mm, and a deep chamfer.28 Before duplication, the prepared tooth was attached to a circular base with 3 rectangular extensions fabricated from a light-polymerized urethane dimethacrylate tray material (Triad; Dentsply Intl). The material increased the diameter of the ivorine tooth shaft to prevent tooth breakage during separation from the silicone mold and to allow sectioning with a low-speed saw (IsoMet speed saw; Buehler Ltd). Polyvinyl siloxane duplicating material (Double Take; Ivoclar Vivodent) was used to make 16 molds of the prepared tooth in a duplicating ﬂask. Type IV dental stone (Resin Rock; Whip Mix Corp) was used to fabricate 80 stone dies from the 16 silicone molds. The stone dies were divided into 5 groups for the 5 die spacer thickness levels: 25 mm, 45 mm, 64 mm, 85 mm, and 105 mm (N=80). A power analysis was completed before the experiment using the mixed models. A statistical analysis was assumed to have been performed for each die
THE JOURNAL OF PROSTHETIC DENTISTRY
Volume 113 Issue 5
Figure 1. A, Cemented coping-die assembly placed under static load of 49 N. B, Low-speed diamond saw with diamond wafering blade. C, Specimen sectioned into halves.
spacer thickness level. Given the die spacer thickness level, 5 measurements for each specimen were treated as repeated measurements to account for within individual correlation. The standard deviation of each measurement was assumed to be 15 and the correlation among the 5 measurements from each specimen to be 0.8. A sample size of 80 (5 locations×16 teeth for each die spacer thickness level) was determined to be sufﬁcient to detect a mean difference of 11 between overall mean (mean of the 5 locations) and the mean of the null hypothesis with 80% power and at a 5% signiﬁcance level. The stone dies were shipped to a commercial laboratory (Nu-Art Dental Inc) for the fabrication of the resin copings. Each die was scanned (D700 3D scanner; 3Shape) according to the manufacturer’s instructions to record the external die form. The 3Shape CAD design system was used to locate the margin and assign the die spacer thickness, which was uniform throughout and terminated 0.5 mm from the ﬁnish line and coping thickness of 1.0 mm.2,5,33 Each resin coping was digitally marked so that it could be paired with its corresponding stone die. The acrylic resin copings were printed (ProJet DP 3000; 3D Systems). The same dental technician at the THE JOURNAL OF PROSTHETIC DENTISTRY
commercial laboratory completed all of the laboratory processes. One dispenser increment volume of self-adhesive resin cement (RelyX Unicem 2; 3M ESPE) was used to cement each printed resin coping to its corresponding die. The cement ﬁlm thickness was determined based on the American Dental Association Speciﬁcation No. 8 protocol, section 220.127.116.11 However, the recommended seating force was reduced to replicate the load used in this experiment (49 N). For the test specimen, the coping was seated with a rocking motion until it was completely seated onto the die. The cemented coping-die assembly was placed under an apparatus capable of maintaining a static deadweight load of 49 N (Fig. 1A), and excess cement was removed with a ﬁne microbrush.35 The mesial, distal, buccal, and lingual surfaces were light polymerized (Demi Plus; Kerr) for 20 seconds each for a total of 80 seconds to ensure complete polymerization. The cemented coping-die assembly was kept under the weightedbase apparatus for 6 minutes. The specimens were stored at room temperature until sectioning. Each specimen was sectioned in a buccolingual direction by using a low-speed diamond saw (IsoMet speed Hoang et al
Figure 3. Microscope image at ×100 magniﬁcation. Indicated are die stone (I), cement layer (II), and resin coping (III).
Table 1. Statistical analysis of accuracy for 5 groups with mixed models Figure 2. Tooth diagram of measured locations. A, Facial chamfer. B, Midfacial axial wall. C, Incisal. D, Midlingual axial wall. E, Lingual chamfer.
saw; Buehler Ltd) with a 127×0.4 mm diamond wafering blade under wet conditions (Fig. 1B). This resulted in 2 specimens for evaluation per coping and die stone (Fig. 1C). The sectioned surface was smoothed with wet 1200-grit silicon carbide paper (MicroCut S; Buehler Ltd) for 1 minute under light pressure. Holmes et al36 deﬁned the internal gap as the perpendicular measurement from the internal surface of the casting to the axial wall of the preparation; the same measurement at the margin was referred to as the marginal gap. The internal gap between the printed resin coping and stone die for each sectioned specimen was measured at 5 deﬁned locations: (A) facial chamfer, (B) facial midaxial, (C) incisal, (D) lingual midaxial, and (E) lingual chamfer (Fig. 2). Five measurements were made to create an average value at each point, leading to a total of 50 measurements (5×2×5) per die.37 Overall, 4000 measurements (50 measurements×80 specimens) were obtained for the entire study. The internal gap image was obtained with an inverted bright ﬁeld metallurgical microscope at ×100 magniﬁcation (Metallograph/Microscope; Leco/Olympus). The microscope was linked to a digital image acquisition device and computer software (Spot v4.5 and v5.1; Spot Image) (Fig. 3). Accuracy was evaluated with mixed model statistical analyses with correlated errors (a=.05). Mixed models were performed for each die spacer thickness level. The paired measurements at the 5 locations per specimen were added as random effect, and the 5 measurements per specimen were treated as repeated measurements within the mixed models to account for correlation within the specimens. The mean of the 5 locations was Hoang et al
Mean Measured (mm)
Mean Difference (mm)
Adjusted P Value Based on FDR (.05)